1 A Comparison of FC-0208 to a 0.3% Molybdenum Prealloyed Low-Alloy Powder with 0.8% Graphite Francis Hanejko Manager, Customer Applications Hoeganaes Corporation Cinnaminson, NJ Abstract Iron copper steels are the most widely used structural PM materials. Although the elemental copper addition melts during initial sintering, complete homogenization of the copper is not achieved at conventional sintering temperatures and sintering times. This lack of microstructural homogeneity coupled with the potential for large pores can often lead to reduced strength and greater dimensional variability during sintering and subsequent heat treatments, if required. A proposed alternative to the FC-02XX materials is a 0.3% molybdenum prealloyed material. This material has nearly identical compressibility compared with the iron copper materials but has the added benefit of a homogeneous microstructure. This paper will focus on a comparison of FC0208 to a 0.3% molybdenum material with 0.8% added graphite. The materials will be compared in both the as-sintered and heat-treated conditions. Additional testing will evaluate the dimensional stability and variability of these two materials in both the as-sintered and heat-treated conditions. Introduction: Iron-copper steels (FC-02XX) are the most widely used structural PM materials. Current applications include main bearing caps, powder forged connecting rods, carrier assemblies, etc. Although FC 02XX series are most frequently used in the as-sintered condition, they are occasionally heat-treated to increase strength or improve wear resistance. One intrinsic drawback of the iron-copper-carbon system is that copper is added elementally. This elemental copper results in part growth during sintering (positive dimensional change, DC) coupled with a potential for large voids after sintering.  A review of the iron copper phase diagram shows that the room temperature solubility of copper in iron is <2% . Nevertheless, production experience shows that large free copper particles are rarely seen in 2% copper steels. Copper contents above 2% show copper precipitates in either the grain boundaries or at prior particle boundaries.
2 Although copper melts at 1083 C (1981 F), the diffusivity of copper into iron is such that complete alloy homogenization is not achieved unless long sintering times or high sintering temperatures are employed. Experimental work by Baran  and Lindsley  illustrated high copper concentrations adjacent to prior particle boundaries with the copper level in the center of the iron particle decreasing to almost zero, see Figure 1. This copper gradient leads to variations in microstructure and a potential for variations in dimensional change (DC) after sintering and heat-treating. Lindsley  demonstrated that this localized gradient causes excessive retained austenite in sinter-hardening grades that can transform to un-tempered martensite upon exposure to low temperature treatments (or low climatic temperatures); thus resulting in additional growth of the component. a. SEM image of 0.50% molybdenum steel with 2% copper added, sintered at 1120 C (2050 F) for 20 minutes at temperature. The line illustrates where both copper and nickel EDAX traces were taken. b. Copper and nickel EDAX traces along scan line in (a.). Note high concentration of copper adjacent to prior particle boundary. Copper trace is shown in green. No nickel was added to this material Figure 1: Copper gradient in a pre-alloyed molybdenum steel, sintered at 1120 C (2050 F) for 20 minutes at temperature The primary advantage of the FC-02XX materials is their unique combination of low material cost coupled with ease of processing and good mechanical properties.  Elemental copper additions do not degrade the base iron compressibility and compacted densities of greater than 7.0 g/cm³ attainable. However, recent developments in the manufacture of low molybdenum content steel powders presents the possibility of substituting a prealloyed 0.3% molybdenum steel powder for the FC02XX materials. With the recent downward trend of molybdenum pricing, the cost penalty of using prealloyed molybdenum steels is lessened. If reductions in part-to-part dimensional variation are possible, then any raw material cost differential will be offset by potential reductions in out of specification parts. This paper will focus on comparing the mechanical properties of an FC-0208 material vs. 0.3% molybdenum steel in both the as-sintered and heat-treated condition. As a second part of this study, the effects of
3 variations in copper and graphite additions were studied to assess the impact of these variables on dimensional change stability and sintered strength. Experimental Procedure: This study was divided into two segments. Part one of the study investigated an FC0208 vs. a prealloyed 0.30% molybdenum steel with 0.8% graphite addition. Part two investigated the sensitivity of variations in copper and graphite additions on the dimensional change of the FC-0208 in relation to variations of graphite additions on the prealloyed 0.3% molybdenum steel. Part 1: Comparison of FC-0208 to 0.3% molybdenum with 0.8% graphite Four premixes were prepared as shown in Table 1. The mixes containing atomized Acrawax C were conventional premixes prepared via double cone blending. The premixes containing the warm die lubricant (AncorMax 200 ) were prepared via a proprietary premixing process. Table 1 Composition of Premixes Prepared for Part 1 Mix Base Iron % Copper % Graphite % Lube & Type 1 Unalloyed iron powder % Acrawax 2 Unalloyed iron powder % warm die lubricant 3 Prealloyed 0.3% % Acrawax Molybdenum 4 Prealloyed 0.3% Molybdenum NA % warm die lubricant The following test specimens were compacted from the four premixes listed in Table 1. Compressibility test specimens at 415, 550, and 690 MPa (30, 40, and 50 tsi). For the warm-die premixes additional compressibility data was generated at 830 MPa (60 tsi). The conventional premixes were compacted in dies at room temperature; whereas, the AncorMax 200 premixes were compacted at 93 C (200 F), no powder preheating. Transverse rupture strength bars for both as-sintered and heat treated strength at the various compaction pressures. MPIF standard dog-bone type tensile specimens for both as sintered and heattreat conditions (MPIF standard 10). Sintering of all samples was done at 1120 C (2050 F) in a continuous belt furnace in an atmosphere of 90% nitrogen / 10% hydrogen for ~20 minutes at temperature; the cooling rate after sintering was ~0.6 C per second (no accelerated cooling). All samples were sintered on ceramic trays. Heat-treated samples were re-austenitized at 815 C (1500 F) in a 75% hydrogen / 25% nitrogen atmosphere for 1 hour at temperature. They were oil quenched in 65 C (150 F) oil and subsequently tempered at 205 C (400 F) for 1 hour in a nitrogen atmosphere.
4 These premixes were utilized to evaluate the dimensional change variability during the heat-treat response of a prototype gear. The gear geometry used is shown in Figure 1. Approximately 1,000 gears were made from each premix, the two conventional doublecone premixes were run in unheated tooling with a target part density of 7.1 g/cm³ and the warm-die lubricant premixes were run in a die heated to 93 C without top punch heating and a target part density of ~7.1 g/cm³. The compacted gears were sintered at 1120 C (2050 F) for 20 minutes at temperature in a 90% nitrogen / 10% hydrogen atmosphere in a 6-inch ceramic belt furnace without accelerated cooling. From these sintered gears 50 were randomly chosen and sent to a commercial heat-treat facility for a quenching and tempering operation. The heat treat cycle used was to austenitize at 870 C (1600 C) for 1 hour in a 0.8% carbon atmosphere followed by oil quenching and tempering. From these 50 heat-treated gears ~20 were then measured for part-to-part dimensional variation via a measurement over wire (MOW) of the gear form. Spur Gear for Evaluation Major OD 1.10 in (28.3 mm) Minor OD 0.85 in (21.6 mm) Pitch Diameter 0.96 in (24.5 mm) Pressure angle 20 ID 0.38 in (9.5 mm) # Teeth 16 Module 1.66 Figure 2: Spur gear produced to evaluate part-to-part consistency in the heattreated condition Part 2: Effect of copper and graphite variations on FC0208 and effect of graphite variations on 0.3% molybdenum prealloy Shown in Table 2 is a list of premixes prepared with the objective of determining the effects of copper and graphite variations on an FC-0208 material and the effects of graphite variations on a 0.3% molybdenum prealloyed steel powder.
5 Table 2 Material Combinations Evaluated to Determine Effects of Copper and Graphite Variations Base Iron w/o Copper w/o Graphite Un-alloyed iron powder Prealloyed 0.3% molybdenum N/A The range shown in Table 2 was selected to cover standard variations in alloy additions that are traditionally used within the FC0208 specification range. All premixes shown in Table 2 were prepared using conventional premixing techniques with 0.75% added Acrawax C. From these premixes, standard transverse rupture strength bars were compacted at 415, 550, and 690 MPa (30, 40, and 50 tsi). Sintering was done under the conditions previously listed. The TRS bars were evaluated for dimensional change and as-sintered strength. Results and Discussion: A. Property comparison of FC-0208 vs. 0.3% prealloyed molybdenum steel with 0.8% graphite Figure 3 presents the compressibility curves of the four materials listed in Table 1. As previously noted, compaction of the Acrawax containing premixes took place in unheated dies at room temperature; whereas, compaction conditions of the warm-die powder premixes was in dies heated to 93 C (200 F) without any prior powder heating. The compressibility of the prealloyed 0.3% molybdenum steel is identical to the FC-0208 material at both room temperature and at die temperatures of 93 C. Utilizing warm die processing results in a 0.05 to 0.10-g/cm³ increase in green density relative to conventional lubricants for both material options. The optimal benefit with warm-die compaction is observed at compaction pressures greater than 550 MPa (40 tsi). Although not shown, warm die processing also promotes higher green strength with reduced green expansion and reduced ejection forces.  The as-sintered and heat-treated transverse rupture strengths as a function of sintered density for the FC0208 and 0.3% molybdenum prealloy with 0.8% added graphite are presented in Figure 4. Warm-die processing did not affect the sintered or heat-treated strength. As anticipated, in the as-sintered condition, the FC-0208 material possesses higher strengths when compared to the prealloyed 0.3% molybdenum material. However, once heat-treated the strengths of the two materials are nearly equivalent.
6 Green Density, g/cm³ FC0208 AM 200 FC % Mo with.8% Gr AM % Mo with.8% Gr Compaction Pressure, MPa Figure 3: Compressibility of the four initial premixes TR Strength, MPa FC0208 as sintered FC 0208 HT A30 HP as sintered A30 HP HT Sintered Density, g/cm³ Figure 4: As-sintered and heat-treated transverse rupture strengths
7 As-sintered tensile properties and heat-treated tensile properties for the 0.8% graphite additions are presented in Table 3. Similar to the trend observed with transverse rupture strength testing, the as-sintered yield and ultimate tensile strengths of the FC-0208 are greater than the prealloyed 0.3% molybdenum steel. Elongation values are nearly the same. Presented in Table 3 are the ultimate tensile strengths of the FC-0208 vs. the 0.3% molybdenum steel in the quenched and tempered condition. Similar to what was found in TRS testing, in the heat-treated condition the prealloyed 0.3% molybdenum steel with 0.8% graphite and heat-treated FC-0208 have nearly identical ultimate tensile strengths. The data presented Table 3 represent compaction at 415, 550, and 690 MPa. The prealloyed 0.3% molybdenum material has lower growth relative to the FC-0208, thus the sintered densities at the same compaction pressure are higher for the prealloyed molybdenum material. Table 3 Summary of Tensile Properties of FC0208 and Prealloyed 0.3% Molybdenum Steel Material FC % Mo Pre-alloy with 0.80% Graphite Sintered Density, g/cm³ Heat Treated 0.2% YS (MPa) UTS, (MPa) Total Elongation (%) Hardness, (HRA) No Yes NA 771 < No Yes NA 805 < B. Dimensional Change and How it is Affected by Variations in Chemistry The dimensional change variations resulting from variations in graphite additions to the two materials studied are studied in Figures 5 and 6. Lowering the graphite addition had an opposite effect for the two materials evaluated. For the FC0208, lowering the graphite to 0.7% had little effect on the DC, remaining approximately the same as the 0.8% additions. However, the 0.30% molybdenum pre-alloyed material with a 0.7% graphite addition showed reduced the DC after sintering. Increasing the graphite to 0.9% resulted in less growth for the FC-0208 relative to 0.8% graphite and approximately the same growth as the 0.8% graphite for 0.3% molybdenum prealloyed steel. The trend observed for the FC-0208 material is consistent with data reported in the literature.  Higher carbon contents in FC0208 material decrease the solubility of copper in iron, thus reducing the growth and increasing the amount of fine copper precipitates.  Conversely, graphite additions above 0.7% result in greater growth for the 0.3% molybdenum prealloyed steel (greater volume expansion of the iron lattice).
8 Sintered DC, % % Cu, 0.80% Gr 2% Cu, 0.70% Gr 2% Cu, 0.9% Gr Green Density, g/cm³ Figure 5: Effect of Graphite additions on the DC of FC Sintered DC, % % Graphite 0.70% Graphite 0.90% Graphite Green Density, g/cm³ Figure 6: Effect of Graphite additions on the DC of 0.3% Molybdenum steel
9 The decrease in growth for FC-0208 with 0.9% graphite was approximately 0.07% to 0.08% over the green density range of 6.75 to 7.10 g/cm³ compared with the material that contained 0.7 or 0.8% graphite. Reviewing the data for the 0.3% molybdenum prealloyed steel, the increase in growth with varying the graphite addition from 0.7% / 0.8% to 0.9% was ~0.05% over the same green density range. Along with reduced scatter, the molybdenum prealloyed steel exhibits reduced growth relative to the FC-0208 material. Another feature of the prealloyed steel material was the reduced growth as a function of increasing green density. The molybdenum steel showed about a 0.05% increase in DC as the density increased from 6.75 to 7.10 g/cm³; while, the FC-0208 material showed ~0.07% increase in growth over the same green density range. Implications of these data are that the molybdenum steel is potentially less sensitive to variations in green density and carbon variations part-to-part. This reduced sensitivity can give reduced part-to-part dimensional scatter and lower heat-treat variations. Interesting for both materials is the overlap of DC for the 0.7% and 0.8% graphite additions for F-C0208 and 0.8% and 0.9% graphite for the 0.3% molybdenum steel. The inference of this is that reduced growth variations can be achieved by maintaining graphite levels in specific (albeit different) ranges for both materials. Sintered DC, % Figure 7: Green Density, g/cm³ Effect of Copper Variations on DC of FC % Cu, 0.8% Gr 2.2% Cu, 0.80% Gr 1.5% Cu, 0.80% Gr 2.5% Cu, 0.80% Gr 2.0% Cu, 0.8% Gr A30HP, 0.8% Gr Shown in Figure 7 is the effect of copper variations on the FC-0208 again comparing the data with the 0.8% graphite molybdenum steel. The data presented in Figure 7 suggest that variations in copper content result in dimensional change variations up to 0.07% over the copper range evaluated. As anticipated variations in both graphite and copper additions result in variability in growth of the FC-0208 material. The absolute magnitude of these variations is larger than the DC variation of the 0.3% molybdenum steel with the potential variability of graphite only.
10 Table 4 Summary of DC Variations for FC-0208 and Pre-alloyed 0.3% Molybdenum Material FC-02XX with 2% Copper 0.3% Mo Prealloy Sintered Density, g/cm³ Heat Treated 0.8% gr 0.9% gr 0.7% gr No Yes No Yes Table 4 presents the maximum variation in DC with variations in graphite content for the alloys tested. A maximum DC variation of ~0.09% can be expected at a given green density with the as-sintered FC-0208 material and the range of graphite additions evaluated in this study. A variation of up to 0.12% was observed for the FC-0208 material in the heat-treated condition. The greatest effect on DC for FC0208 materials results from variations in graphite additions. For the molybdenum pre-alloyed steel at a given density level; potential variations in carbon content result in a maximum DC variation in the as-sintered condition of ~0.08%. Heat-treating the molybdenum steel reduces this maximum DC variation to ~0.04% (approximately one third of the variation observed with the FC-0208). Sintered and heat treated TRS testing of materials with the possible variations in copper / graphite for the FC-0208 and for graphite only for the 0.3% molybdenum steel are shown in Table 5. Focus is given to TRS results only. Copper has the strongest influence on TRS properties for copper containing steels. Higher copper contents increase TRS strength; this results from additional precipitation hardening effects. Results for the 0.3% molybdenum steel show the highest heat-treated strength with a graphite addition of 0.7%. Additional graphite decreases the strength. A possible explanation for these phenomena is that molybdenum is a ferrite stabilizer and it decreases the eutectoid carbon level. At graphite additions of 0.8% and 0.9% the occurrence of grain boundary carbides are possible.
11 Table 5 Range of Sintered and Heat-Treated TRS Test Results for Copper and Graphite Variation Iron Base % Cu % Gr Unalloyed Iron 0.30% molybdenum prealloy steel NA Sintered Density, g/cm³ Sintered TRS, MPa (psi) Heat Treated TRS, MPa (psi) (133,700) 1100 (160,000) (150,500) 1305 (189,600) (167,600) 1325 (192,600) (123,600) 1100 (160,000) (153,100) 1340 (194,600) (170,500) 1450 (210,500) (113,000) 990 (143,800) (139,300) 1195 (173,500) (156,100) 1240 (180,500) (97,900) 1055 (153,100) (119,000) 1370 (198,900) (132,200) 1480 (215,350) (98,000) 1120 (163,000) (119,000) 1205 (175,300) (132,000) 1295 (187,900) (104,600) 940 (136,100) (124,700) 1130 (163,800) (134,100) 1215 (176,900) C. Results of heating treating gear shown in Figure 2. Prototype gears were produced using the four materials discussed in part one of this study. They were made on a Dorst 140 metric ton compaction press at a rate of 10 per minute. The gears were sintered in a continuous belt sintering furnace at 1120 C (2050 F) in a 90% nitrogen / 10% hydrogen atmosphere with a time at temperature of ~20 minutes. After sintering approximately 50 gears from each material grouping were heattreated by quenching and tempering utilizing a commercial heat-treat cycle for FC0208. After quenching, the gears were then tempered at 205 C (400 F). The gears were checked for dimensional variation using mm ( inch) diameter pins. Measurements were taken at four locations per gear starting with the front of the gear (as compacted) and then measuring three additional locations around the outside diameter. The results of the measurement over wires (MOW) are presented in Table 6.
12 Table 6 Dimensional Variations of Heat Treated Gears Material FC-0208 (regular premix) 0.3% Mo with 0.8% gr (regular premix) FC-0208 (bonded premix 0.3% Mo with 0.8% gr (bonded premix) Av. MOW Inches (mm) (30.72) (30.71) (30.73) (30.69) Max MOW Inches (mm) (30.78) (30.72) (30.78) (30.71) Min MOW Inches (mm) (30.67) (30.69) (30.69) (30.67) Max Min Inches (mm) (0.11) (0.04) (0.09) (0.04) St Dev MOW (0.03) (0.01) (0.02) (0.01) Table 7 Apparent Hardness Values of Gears in the Heat-Treated Condition Material FC-0208 (regular premix) 0.3-0% Mo with 0.8% gr (regular premix) FC-0208 (bonded premix 0.3% Mo with 0.8% gr (bonded premix) Sintered Density, g/cm³ Average Hardness, HRA Range of Hardness, HRA / / / / 73.5 The data presented in Table 6 clearly demonstrate the reduced scatter realized with the prealloyed 0.3% molybdenum steel relative to a standard FC-0208 material. The absolute magnitude of the MOW is different for the two material combinations; this is a result of the absolute DC differences between an FC-0208 and a 0.3% molybdenum prealloyed steel with 0.8% graphite. Thus, it can be clearly seen that a molybdenum steel gives greater dimensional stability in the heat-treated condition. No green or sintered gears were measured because the focus of this report was to investigate heattreated results. One additional observation is the comparison of the warm-die powder premixes vs. regular premixes. For the FC-0208 material, the binder treated warm-die powder gave a reduced overall scatter as measured by the maximum measurement minus the minimum measurement and also the standard deviation of the measurement differences. Thus, the binder treatment does result in reduced part-to-part scatter even
13 for the copper-containing steel. No difference in dimensional variation was observed for the binder treated 0.3% molybdenum steel. Apparent hardness data collected on the gears are presented in Table7. The gears were initially compacted to a 7.1 g/cm³ green density; the densities given in the table are heat-treated densities. Another benefit of the low alloy steel powder is the greater uniformity of heat-treated hardness as measured by the range of hardness readings. One potential benefit of eliminating the copper may be a reduced tendency for cracking during induction hardening. Induction hardening of copper containing PM steels has shown sensitivity to cracking. A possible explanation is the non-uniform microstructure inherent with copper containing PM steels. Eliminating the copper would eliminate one potential for crack initiation during induction hardening of the PM materials. Discussion: The objective of this study was to evaluate the feasibility of using a 0.3% molybdenum steel in lieu of FC In the as-sintered condition, the TRS and tensile properties of the 0.3% molybdenum steel with 0.8% graphite are inferior to the FC-0208 steel. The molybdenum steel does experience less growth during sintering compared with the FC Additionally, the molybdenum prealloyed steel has reduced DC variation resulting from variations in compacted density and premixed graphite variations when compared to the copper steel. Once heat-treated the 0.3% molybdenum steel with 0.8% graphite has nearly equivalent TRS and ultimate tensile strength compared to the copper steel. Dimensional change of the heat-treated TR specimens using the molybdenum steel exhibited reduced dimensional change variation with variations in density and variations in graphite additions. An implication of this data suggests that reduced scatter is possible in actual components that required a heat-treatment. Measurement over wire measurements of compacted, sintered, and heat-treated gears showed a significant reduction in the variability of the MOW within a gear and gear measurements made over 20 measured gears. This reduced variation as measured by the standard deviation of the MOW was greater than 50%. One possible implication of this data is the potential to use a 0.3% molybdenum prealloyed steel in those applications possessing tight dimensional control coupled with a heat-treated microstructure. PM is continually being challenged to produce evertighter DC along with higher densities. Using a prealloyed molybdenum steel reduces variations in DC with variations in density and graphite levels yet provides heat-treated strengths equivalent to heat-treated FC Additionally, the uniform microstructure promotes greater uniformity of hardness with the potential for reduced cracking if induction hardening is required. Conclusions: Results from this study showed the following trends: 1. In the as-sintered condition an FC-0208 has superior mechanical properties when compared with a 0.3% molybdenum prealloyed steel with 0.8% added graphite.
14 2. In the heat-treated condition, the 0.3% molybdenum prealloyed steel with 0.8% added graphite has nearly identical strength to a heat treated FC Variations in graphite additions have opposite effects on both material. Higher graphite additions result in less growth for the FC-0208 and approximately the same growth for a 0.3% molybdenum prealloyed steel. 4. Reducing the graphite addition to 0.7% results in more growth for the FC-0208 and less growth for the 0.3% molybdenum prealloyed steel. 5. Carbon has the greatest effect on DC variation for the copper steels. 6. Variations of part density result in lower DC variations for the 0.3% molybdenum pre-alloyed material when compared with the FC Heat treatment of gears made from both materials showed greater dimensional scatter for a FC-0208 relative to a 0.3% molybdenum prealloyed steel. 8. Using a binder treated FC-0208 resulted in reduced scatter relative to a regular premix. The rationale for this is the reduced potential for graphite segregation. References: 1. ASM Metals Handbook, Volume 7 Ninth Edition, published by ASM International, Materials Park, Ohio, 1998, pp ASM Metals Handbook, Volume 8 Eight Edition, published by ASM International, Materials Park, Ohio, 1973, p T. Murphy, M. Baran, An Investigation into the Effect of Copper and Graphite Additions to Sintering Hardening Grades Advances in Powder Metallurgy and Particulate Materials --, Compiled by W. Brian James and Russell A. Chernenkoff, Metal Powders Industries Federation, 2004, pp. 4. B. Lindsley, T. Murphy, Effect of Post Sintering Thermal Treatments on Dimensional Precision and Mechanical Properties of Sinter Hardening PM Steels, Advances in Powder Metallurgy and Particulate Materials , Compiled by John Engquist and Thomas F. Murphy, Metal Powders Industries Federation, 2007, pp.. 5. Materials Standards for PM Structural Parts, MPIF standard 35, 2007 Edition, published by Metal Powders Industry Federation, Princeton, NJ, 2007, pp F. Hanejko, High Density via Single Pressing / Single Sintering, Presented at Euro PM Hoeganaes Corporation Technical Literature at product, unalloyed steels.
EFFECT OF COPPER ALLOY ADDITION METHOD ON THE DIMENSIONAL RESPONSE OF SINTERED FE-CU-C STEELS Michael L. Marucci and Francis G. Hanejko Hoeganaes Corporation Cinnaminson, NJ 08077 - USA Abstract Fe-Cu-C
Development of a High Performance Nickel-Free P/M Steel Bruce Lindsley Senior Materials Engineer, Hoeganaes Corporation, Cinnaminson, NJ 08077, USA Abstract A developmental nickel-free P/M steel containing
Full Density Properties of Low Alloy Steels Michael L. Marucci & Arthur J. Rawlings Hoeganaes Corporation, Cinnaminson, NJ Presented at PM 2 TEC2005 International Conference on Powder Metallurgy and Particulate
% of Graphite Bonded % of Lubricant Bonded % of Copper Bonded Improved Powder Performance Through Binder Treatment of Premixes C.T. Schade 1 and M. Marucci 1 1 Hoeganaes Corporation, 1001 Taylors Lane,
Effect of Small Additions of Boron on the Mechanical Properties and Hardenability of Sintered P/M Steels Michael Marucci *, Alan Lawley **, Robert Causton *, and Suleyman Saritas *** * Hoeganaes Corporation,
ADVANCED PERFORMANCE ALLOYS PROCESSED BY HIGH TEMPERATURE SINTERING TECHNIQUE Patrick King and Michael Marucci Hoeganaes Corporation, Cinnaminson, NJ Bill Edwards, Leonid Frayman, Dax Whitehouse, Ron Payne
IMPACT AND FATIGUE CHARACTERIZATION OF SELECTED FERROUS P/M MATERIALS Robert C. O'Brien Hoeganaes Corporation River Road Riverton, New Jersey 08077 Presented at the Annual Powder Metallurgy Conference,
CHARACTERISTICS OF IRON AND STEEL POWDERS The most important prerequisite of a successful mass production of high-quality sintered parts is a high and consistent quality of the powder from which the parts
2002-01-0670 Materials Solutions for Converting Cast Iron Applications to Powder Metal Michael C. Baran and K.S. Narasimhan Hoeganaes Corporation Copyright 2002 Society of Automotive Engineers, Inc. ABSTRACT
PM Steels That Contain Manganese Bruce Lindsley and Brian James Hoeganaes Corporation Cinnaminson, NJ 08077, USA ABSTRACT The ferrous PM industry continues to develop and expand its use of non-traditional
FATIGUE PROPERTIES OF P/M MATERIALS Robert C. O'Brien Hoeganaes Corporation River Road Riverton, New Jersey 08077 Presented at the SAE Congress Detroit, Michigan, February 29-March 4, 1988 Abstract The
CHROMIUM STEEL POWDERS FOR COMPONENTS JEANETTE LEWENHAGEN Höganäs AB, Sweden KEYWORDS Pre-alloyed steel powder, chromium, PM ABSTRACT Chromium as an alloying element is of great interest due to its low
s 410, 420, 425 Mod, and 440A GENERAL PROPERTIES s 410, 420, 425 Modified, and 440A (see composition on Page 2) are hardenable, straight-chromium stainless steels which combine superior wear resistance
PRECIPITATION HARDENING P/M STAINLESS STEELS Chris Schade, Pat Stears Hoeganaes Corporation Cinnaminson, NJ 08077 Alan Lawley, Roger Doherty Drexel University Philadelphia, PA 19104 ABSTRACT Applications
WHAT IS SINTER-HARDENING? W. Brian James Abstract Hoeganaes Corporation Cinnaminson, NJ 08077 Presented at PM 2 TEC '98 International Conference on Powder Metallurgy & Particulate Materials May 31 - June
Abstract HIGH DENSITY PROCESSING OF HIGH PERFORMANCE FERROUS MATERIALS H. G. RUTZ and F. G. HANEJKO HOEGANAES CORPORATION RIVERTON, NJ 08077 PRESENTED AT 1994 INTERNATIONAL CONFERENCE & EXHIBITION ON POWDER
COLD PRESSING POWDER WITH ASSISTED FRICTION COMPACTION FOR HIGH-SPEED TOOL STEELS I.M. Sas-Boca, T. Canta, D. Frunza Engineering and Materials Processing Department, Technical University of Cluj-Napoca,
COMPARISON OF MASTER ALLOY AND PRE-ALLOYED 316L STAINLESS STEEL POWDERS FOR METAL INJECTION MOLDING (MIM). Paul A. Davies and G. R. Dunstan Powder Group, Sandvik Osprey Ltd Neath, United Kingdom SA11 1NJ
MARTENSITIC STAINLESS STEEL RWL-34 RWL 34 is a Rapid Solidified Powder (RSP) Martensitic Stainless Steel, which is variation of the 420 martensitic stainless steel family with minimum 13 percent chromium
Test Device and Method for Evaluation of Lubricants for P/M Compaction Gerald A. Gegel Engineering Specialist-Research Caterpillar Inc. Dr. Sydney Luk Director, Chemical Technologies Hoeganaes Corporation
Training Objective After watching the program and reviewing this printed material, the viewer will gain a knowledge and understanding of the basics of powder metallurgy. Types of particles are explained.
ATI 316Ti Stainless Steel: Austenitic (UNS S31635) GENERAL PROPERTIES ATI 316Ti stainless is a titanium-stabilized version of Type 316 molybdenum-bearing austenitic stainless steel. It is also known as
STAINLESS STEEL AISI GRADES FOR PM APPLICATIONS Chris Schade Hoeganaes Corporation Cinnaminson, NJ 08077 John Schaberl Ancor Specialties Ridgway, PA 15853 Alan Lawley Drexel University Philadelphia, PA
Post-Weld Heat Treatment Case Studies Khaleel Ahmed and J. Krishnan Centre for Design and Manufacture Bhabha Atomic Research Centre Introduction H EAT TREATMENT IS AN IMPORTANT operation in the final fabrication
SOFT MAGNETIC MATERIAL FOR A.C. APPLICATIONS Author(s): Kalathur Narasimhan, Francis Hanejko, Michael L. Marucci Hoeganaes Corporation Abstract Soft magnetic material using powder metallurgical techniques
Technical Data BLUE SHEET Allegheny Ludlum Corporation Pittsburgh, PA Martensitic Stainless Steels Types 410, 420, 425 Mod, and 440A GENERAL PROPERTIES Allegheny Ludlum Types 410, 420, 425 Modified, and
Martensitic stainless RWL 34 Damasteel s martensitic stainless RWL 34 is a Rapid Solidified Powder (RSP) based steel which is a variation of the 420 martensitic stainless steel with > 13 % Chromium. The
Indu UR 317L UR 317L: A 3%Mo minimum austenitic stainless (317L grade) UR 317L (317L) is an austenitic stainless with a 3% molybdenum addition. Alloy UR 317L (317L) exhibits an austenitic microstructure,
Controlling Properties of Sintered Steel Powder Metal Components Using Atmosphere Composition as a Variable Thomas Philips, John J. Dwyer, Jr. and Zbigniew Zurecki Air Products and Chemicals, Inc. 7201
Module 4 Design for Assembly Lecture Design for Heat Treatment 7 Instructional objectives By the end of this lecture, the student will learn 1. different heat treatment processes, 2. application of various
HIGH PERFORMANCE LUBRICANTS FOR DEMANDING PM APPLICATIONS Sylvain St-Laurent, Yannig Thomas * and Lhoucine Azzi * Quebec Metal Powders Limited Tracy, Québec * Industrial Materials Institute, National Research
Proceedings of COBEM 2009 Copyright 2009 by ABCM 20th International Congress of Mechanical Engineering November 15-20, 2009, Gramado, RS, Brazil INFLUENCE OF DELTA FERRITE ON MECHANICAL PROPERTIES OF STAINLESS
SINTERING OF POWDER PREMIXES A BRIEF OVERVIEW Kalathur S.Narasimhan and Frederick J.Semel Hoeganaes Corporation 1001 Taylors lane Cinnaminson,NJ 08077 Abstract Advances in the understanding of the sintering
International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 28-32 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia
Problem Set 7 Materials101 1.) You wish to develop a gold alloy (mostly gold) that can be precipitation strengthened to provide high strength - high conductivity electrical leads to integrated circuits
DH31-EX!!! NADCA Approved 2011 Ultra High Strength, tough, and high heat check resistance hot work die steel. DH31-EX, produced exclusively by Diado Steel Ltd., is a hot working die steel with the best
NiDI Nickel Development Institute Nickel in powder metallurgy steels A Nickel Development Institute Reference Book, Series N 11 006 Foreword Nickel has found an important place as an alloying element in
North American Stainless Flat Products Stainless Steel Grade Sheet 310S (S31008)/ EN 1.4845 Introduction: SS310 is a highly alloyed austenitic stainless steel designed for elevated-temperature service.
TM A high hardness, corrosion and fatigue resistance martensitic grade CONTINUOUS METALLURGICAL SPECIAL STEELS INNOVATION RESEARCH SERVICE DEVELOPMENT Enhancing your performance THE INDUSTRIAL ENVIRONMENT
Euro PM2003 High Alloy Steels Iron Based Materials With Improved Oxidation Resistance Prepared By Powder Metallurgy Thomas Weissgaerber; Lothar Schneider; Bernd Kieback Fraunhofer-Institute for Manufacturing
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature
North American Stainless Long Products Stainless Steel Grade Sheet 2205 UNS S2205 EN 1.4462 2304 UNS S2304 EN 1.4362 INTRODUCTION Types 2205 and 2304 are duplex stainless steel grades with a microstructure,
Introduction to Metallography Metallography has been described as both a science and an art. Traditionally, metallography has been the study of the microscopic structure of metals and alloys using optical
As seen in the September/October 1999 issue of Gear Technology Cast Iron: A Solid Choice for Reducing Gear Noise Robert O'Rourke Robert O'Rourke is a product engineering manager with the Dura-Bar division
Data Sheet: A2.2 High carbon and quenchable steels Hot Rolled Steel Plate and Coil for Hardening and Wear Resistance General description Steel is generally classified as high carbon steel if the nominal
Introduction to Iron Metallurgy Lee Morin Houston Home Metal Shop Club October 2010 Book I stole the pictures from We will start with a brief overview! Metals Are Crystals Fundamental geometry of a crystal
INDUSTRIAL MATERIALS Development of High-Strength Steel Wire with Superior Weldability Hiromu IzumIda*, Kenichi SHImIzu, Shinei TaKamura, Yasuhiro SHImoda, osamu momozawa and Teruyuki murai High-carbon
MPIF Standard 35 s Standards for Metal Injection Molded Parts Issued 1993 Revised 2000 and 2007 Scope MPIF Standard 35 is issued to provide the design and materials engineer with the information necessary
HEAT TREATMENT OF STEEL Heat Treatment of Steel Most heat treating operations begin with heating the alloy into the austenitic phase field to dissolve the carbide in the iron. Steel heat treating practice
Heat Treatment of Steel Steels can be heat treated to produce a great variety of microstructures and properties. Generally, heat treatment uses phase transformation during heating and cooling to change
Outline: I.Introduction Where used Advantages/Disadvantages (limitations) Material Properties II. The P/M Manufacturing Process Production of Metal Powders Compaction Sintering Secondary Operations II.
Part VI. : Heat treatment Module 5 : Some standard heat treatments 5 Some standard heat treatments 5.1 Annealing Consider the TTT diagram as shown in Fig. 9 and the cooling curves imposed on the TTT diagram.
Development of Metal Injection Molding Process for Aircraft Engine Part Production IKEDA Shuji : Manager, Engine Technology Department, Research & Engineering Division, Aero-Engine & Space Operations SATOH
Evaluation of the Susceptibility of Simulated Welds In HSLA-100 and HY-100 Steels to Hydrogen Induced Cracking R. E. Ricker, M. R. Stoudt, and D. J. Pitchure Materials Performance Group Metallurgy Division
ALLOY 2205 DATA SHEET UNS S32205, EN 1.4462 / UNS S31803 GENERAL PROPERTIES ////////////////////////////////////////////////////// //// 2205 (UNS designations S32205 / S31803) is a 22 % chromium, 3 % molybdenum,
North American Stainless Long Products Stainless Steel Grade Sheet AISI 310S S31008 EN 1.4845 AISI 314 S31400 EN 1.4841 INTRODUCTION Types 310S SS and 314 SS are highly alloyed austenitic stainless steels
Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.
CONSOLIDATION AND HIGH STRAIN RATE MECHANICAL BEHAVIOR OF NANOCRYSTALLINE TANTALUM POWDER Sang H. Yoo, T.S. Sudarshan, Krupa Sethuram Materials Modification Inc, 2929-P1 Eskridge Rd, Fairfax, VA, 22031
International Journal of Engineering Research and Technology. ISSN 0974-3154 Volume 6, Number 6 (2013), pp. 767-772 International Research Publication House http://www.irphouse.com Properties and Welding
AUSTENITIC STAINLESS DAMASCENE STEEL Damasteel s austenitic stainless Damascene Steel is a mix between types 304L and 316L stainless steels which are variations of the 18 percent chromium 8 percent nickel
Metal Injection Molded Parts Metal Injection Molding (MIM) is a powder metallurgy process. he difference between MIM and conventional powder metallurgy is that in MIM, metal powder along with binders is
Heat Treatment of Steels :Recrystallization annealing The carbon and alloy steels were treated at a temperature of about 700 C, which is about 20 C below the eutectoid temperature. The holding time should
Introduction: North American Stainless Flat Products Stainless Steel Grade Sheet 309S (S30908)/ EN1.4833 SS309 is a highly alloyed austenitic stainless steel used for its excellent oxidation resistance,
Chiang Mai J. Sci. 2006; 33(1) : 53-66 www.science.cmu.ac.th/journal-science/josci.html Contributed Paper Density and Strength Improvement of Sintered 316L Stainless Steel Nattaya Tosangthum*, Ornmanee
April 29 th 2015 THE MICROSTRUCTURE AND PROPERTIES OF HOT PRESSED IRON BRONZE POWDERS BOROWIECKA-JAMROZEK Joanna Department of Applied Computer Science and Armament Engineering, Faculty of Mechatronics
Damasteel s martensitic stainless Nitrobe 77 is a powder based steel which solves two classical knife problems: Sharp edges on chef knives. Nitrobe 77 is dishwasher safe without risk of corrosion or edge
Comparison of Three Ni-Hard I Alloys Ö. N. Do an 1, J.A. Hawk 1, and J.Rice 2 1 U.S. Department of Energy, Albany Research Center, Albany, Oregon 2 Texaloy Foundry Co., Inc., Floresville, Texas Keywords:
Standard Specification for Wrought High Strength Ferritic Steel Butt Welding Fittings 1. Scope :- 1.1 This specification covers wrought high strength ferritic steel butt-welding fitting of seamless and
Page 1 of 5 MEEHANITE SELECTION GUIDE Presented by Lodi Iron Works, Inc 1-888-368-5395 General Engineering Applications Meehanite Flake Graphite Types -Type AQ is a wear and abrasion resisting iron that
Girish P. Kelkar, Ph.D. (562) 743-7576 firstname.lastname@example.org www.welding-consultant.com Weld Cracks An Engineer s Worst Nightmare There are a variety of physical defects such as undercut, insufficient
1 POSSIBILITY OF INDIRECT HARDNESS TESTING OF DUPLEX STAINLESS STEEL István Mészáros Associate professor, Department of Materials Science and Engineering H-1111 Budapest, Goldmann tér 3. Summary In this
Unit Display: English D2 Tool Steel UNS Number T30402 AISI Number Type D2 Identification Print Now E-Mail Datasheet Add to My Materials Type Analysis Carbon 1.50 % Manganese 0.50 % Silicon 0.30 % Chromium
HOT-WORK TOOL STEELS WITH IMPROVED PROPERTIES FOR DIE CASTING APPLICATIONS K.-D. Fuchs Edelstahl Witten-Krefeld GmbH Quality Department Tool Steel Auestraße 4 D-58452 Witten Abstract Keywords: To get a
THE WAY TO SOMEWHERE Sub-topics 1 Diffusion Diffusion processes in industry RATE PROCESSES IN SOLIDS At any temperature different from absolute zero all atoms, irrespective of their state of aggregation
Friction Stir Welding of Stainless Steel and Nickel Base Alloys R.J. Steel, T.W. Nelson, C.D. Sorensen, Y.S. Sato, C.J. Sterling, and S.M. Packer Acknowledgements Material provided by: Haynes International
Weld Cracking An Excerpt from The Fabricators' and Erectors' Guide to Welded Steel Construction The James F. Lincoln Arc Welding Foundation Weld Cracking Several types of discontinuities may occur in welds
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
Laser Welding P/M For Automotive Applications SAE Technical Paper 940355 Jack A. Hamill, Jr. Hoeganaes Corp. Peter Wirth Rofin-Sinar, Inc. Presented at the SAE International Congress and Exposition February
High Strength Steel (HSS) tubes for structural and engineering applications 2 Tenaris produces a large dimensional range of seamless tubes in high strength steel for engineering and structural applications
1 2 Selecting the proper Tool Steels, Heat Treatment, & Surface Treatments for a stamping application can be a complex and confusing process. To simplify this process, a few basic facts should be understood.
STAVAX SUPREME Stainless tool steel General Demands placed on plastic mould tooling are increasing. Such conditions require mould steels that possess a unique combination of toughness, corrosion resistance
Plastic Behaviour - Tensile Strength Transition of mechanical behaviour from elastic to plastic depends upon the material type and its condition as tested (hot-rolled, cold-rolled, heat treated, etc.).
Available on line at Association of the Chemical Engineers AChE www.ache.org.rs/ciceq Chemical Industry & Chemical Engineering Quarterly 15 (3) 131 136 (2009) CI&CEQ ZORAN JANJUŠEVIĆ ZVONKO GULIŠIJA MARIJA
Journal of Metals, Materials and Minerals, Vol.23 No.2 pp.1-7, 2013 Heat treatment of steel parts in different media Suresh C. MAIDARGI and Veena RANI* Department of Chemical Engineering, Dayananda Sagar
FEATURES AND BENEFITS OF DIFFERENT PLATINUM ALLOYS Kris Vaithinathan and Richard Lanam Engelhard Corporation Introduction There has been a significant increase in the world wide use of platinum for jewelry
9-2 9.2 (a) From Figure 9.8, the maximum solubility of Pb in Sn at 100 C corresponds to the position of the β (α + β) phase boundary at this temperature, or to about 2 wt% Pb. (b) From this same figure,
Journal of Minerals & Materials Characterization & Engineering, Vol. 11, No.2 pp.143-152, 2012 jmmce.org Printed in the USA. All rights reserved Effect of Heat Treatment Processes on the Mechanical Properties